(2) Design of Reflective, Photonic Shields for Atmospheric Reentry. make omnidirectional RPS for other wavelength ranges as well. The advantage of the proposed one-dimensional structures is that they are relatively simple to model and to fabricate. The constituent materials silicon dioxide SiO 2 and zirconium dioxide ZrO 2 are chosen. These materials meet a number of the strict requirements of this application, such as high-temperature stability, low absorptivity, oxidation resistance and others. However, the SiO 2 ZrO 2 couple has small dielectric contrast, making the design of a omnidirectional RPS more difficult than for materials with a higher dielectric contrast. This paper is organized as follows. In Section 2, the optimization model of an omnidirectional RPS appropriate for two energy intervals is defined. Next, in Section 3, we apply a band gap analysis to SiO 2 ZrO 2 periodic multilayers and construct an omnidirectional RPS in the desired energy intervals. By combining (stacking) different periodic segments in one structure a high reflectivity can be achieved. In Section 4, we briefly discuss different optimizers, which are applicable for the optimization of layered structures. As an example, we optimize the omnidirectional reflectivity of a layered structure using ES and compare our results with the Bragg and optimized Bragg mirrors. Then, in Section 5 optimization of the RPS for either to B1 or to B2 energy interval is performed. The optimization of the RPS for both energy intervals is performed in Section 6. Finally, in Section 7, changes of in the multilayer structure due to high temperature interdiffusion and the possible consequences on reflecting properties of RPS are discussed.. 2. Definition of the Problem The RPS for Earth reentry should be optimized for energy intervals B1 and B2 and should possess omnidirectional reflectivity. The energy ranges for B1 and B2 are 1 - 2 eV ( 650 - 1200 nm) and 2.4 - 4.2 eV ( 300 - 500 nm) respectively. We have chosen silicon dioxide SiO 2 and zirconium dioxide ZrO 2 as the materials for the individual layers. Silicon dioxide and zirconium dioxide have high melting temperatures Tm = 1650˚C and Tm = 2715˚C respectively and are optically transparent in the ranges of interest. SiO 2 (quartz) and ZrO 2 have similar coefficients of thermal expansions. The high-temperature interaction of SiO 2 and ZrO 2 layers results in the formation of a high-temperature stable phase of ZrSiO4 which may have possible diffusion barrier properties (see Section 7). This phase may prevent further Si and Zr interdiffusion, and therefore result in reduction of photonic properties. Permittivity data of the materials are shown in Figure 2. Both materials are dielectrics with a wide gap, so we assume that Copyright © 2011 SciRes.. 229. permittivity should not strongly change with temperature. However, all calculations are performed with permittivity values at room temperature, since data for permittivity at high temperature are not available. Basic properties for possible candidate materials for high-temperature photonic applications are given in Table 1. Our goal is to design a layered structure which maximizes the percentage of reflection R of unpolarized electromagnetic radiation within two energy intervals for a fixed number of layers N. Therefore, we define a fitness function as the average reflection in two energy intervals:. Fitness = R d1 , d 2 , , d N =. R1 R2 1, 2. (1). Figure 2. Permittivity of SiO2 and ZrO2 from . Table 1. Melting points (Tm), dielectric permittivity , and density of some possible materials for the high temperature photonics. Material. Tm ,˚C. , Ref. . , g cm 3. MgO. 2825. 3.7 0.6i (at 1 μm). 3.6. Y2O 3. 2440. 3.6 (at 1 μm). 5.0. Al2O3. 2050. 2.7 (at 1 μm). 4. TiO 2. 1840. 7.5 (at 1 μm). 4.2. SiO 2. 1650. 2.1 (at 1 μm). 2.2. ZrO 2. 2715. 4.8 (at 0.8 μm). 5.9. HfO 2. 2800. 3.6 (at 0.8 μm). 9.7. MgF2. 1260. 1.9 (at 0.8 μm). 3.1. SiC. 2830. 6.8 (at 1 μm). 3.2. Si 3 N 4. 1900. 4 (at 1 μm). 3.2. Nb 2O5. 1500. 4.4 (at 1 μm) Ref. . 4.5. JEMAA.
(3) Design of Reflective, Photonic Shields for Atmospheric Reentry. 230. R1,2 =. 1 Rs , Rp , dd 2 1.2 . dd. 1,. (2). 1.2 . where Rs and Rp are the reflection coefficients for s(electric field parallel to layers) and p-polarized (magnetic field parallel to layers) light respectively and are π integrated over the angles of incidence 0, and 2 energy intervals 1 1, 2 , 2 2.4, 4.2 eV. The thickness of the i-th layer ( i = 1, , N ) is di . We need to maximize the function R d1 , d 2 , , d N of N variables, which are layer thicknesses. Moreover, the obtained solution should also be robust. This implies that reflection R does not vary strongly with small deviation of layer thicknesses di . In other words, unavoidable fabrication inaccuracies of layer thicknesses should not significantly change reflecting performance of the structure.. band gap for p-polarized light becomes narrower for the inclined incidence light as can be seen in the plot. Since point B is slightly above point C, the structure has no omnidirectional reflection. In order to circumvent the difficulty of narrow gaps,. 3. Design of the RPS Using Photonic Band Gap Approach Construction of omnidirectional mirrors from layered media were analyzed and discussed in many works [8-10]. There are two necessary requirements to achieve omnidirectional reflection. The first is a sufficiently high dielectric contrast for the constituent materials. The second is that the dielectric constant of the lower index material is larger than the dielectric constant of the ambient medium by some critical amount. Reflection in a broader energy interval can be achieved by stacking several periodic layered media with different periods . Another way to achieve reflection in a broad range is to use a chirped periodic layered medium [11,12]. Other optimization procedures, like the quasi-Newton algorithm  or genetic algorithms [14,15] have also been applied to improve the performance of finite multilayer mirrors. Let us consider an infinitely-periodic structure consisting of SiO 2 and ZrO 2 layers. The geometry is shown in Figure 3(a) For normal incidence light k x = 0 . the gap-midgap ratio is maximized when d1n1 = d 2 n2 (quarter wave stack condition). For grazing incidence k x c , the gap-midgap ratio is maximized when. (a). d1 n12 1 = d 2 n22 1 .. The main difficulty in designing a RPS with sufficiently broad band gaps for both B1 and B2 energy intervals is the low dielectric contrast of SiO 2 and ZrO 2 materials. A simple periodic Bragg mirror is not a suitable solution, because the band gaps are narrow and not omnidirectional. The band structure of a Bragg mirror with period = 425 nm is shown in Figure 4. The Copyright © 2011 SciRes.. (b). Figure 3. (a) Multilayer SiO2/ZrO2 with period constant through the whole stack, d1,2 and n1,2 are thicknesses and refractive indexes of the layers respectively. (b) Multilayer stack consisting of segments with different periods. Angle of light incidence is , k = k x , 0, k z is the wave vector. JEMAA.
(4) Design of Reflective, Photonic Shields for Atmospheric Reentry. Figure 4. Band structure of SiO2/ZrO2 Bragg mirror with period 425 nm for s- and p-polarized light. White region between shadowed regions corresponds to band gap. Solid black line denotes air light cone, dashed and dash-dotted lines denote Brewster’s cones of SiO2/ZrO2 and air/ZrO2 interfaces respectively (ZrO2 is on top of structure).. we can stack segments with different periods, as shown in Figure 3(b). If the periods of the segments are chosen appropriately, then the total omnidirectional band gap can include the entire desired energy range. As can be concluded from Figure 4, the condition for band gap overlapping in p-polarization is that point B of the next segment with a smaller period should be slightly below point A of the previous segment with a larger period. Band gap overlapping in s-polarization is automatically fulfilled using this criteria. In order to generate an omnidirectional gap in the first range (1 - 2 eV) we need ten periodic segments with uniformly spaced periods from 200 to 425 nm. The band structure of ten segments is shown in one of the plots in Figure 5(a). Note that the B2 range 2.4 - 4.2 meV is already significantly covered with band gaps of higher orders. This means that reflection of finite structure for the B2 range will also be high. However, in order to completely cover the B2 range with first order gaps, we need eight additional segments with uniformly spaced periods from 90 to 180 nm. The resulting band structure is shown in Figure 5(b). Thus, a total of 18 segments are required to cover both B1 and B2 energy intervals with band gaps. The magnitude of Im k z in Figure 5 determines the rate of exponential decay of the propagating wave and also affects the reflectivity of the structure. As seen in the plot, the magnitude of Im k z is larger for higher energies (or smaller periods of segments) in both B1 and B2 ranges. However, the product Im k z remains constant for all periods in the segments. Therefore, we take equal numbers of layers in each of the 18 segments. Calculations of the reflectivity of these stacked segments are discussed in Sections 5 and 6. Copyright © 2011 SciRes.. 231. (a). (b). Figure 5. (a) Band structure of ten segments with uniformly spaced periods from 200 to 425 nm shown in one plot. The total omnidirectional band gap is in the B1 energy interval 1 - 2 eV. (b) Band structure of eight segments with uniformly spaced periods from 90 to 180 nm shown in one plot. The total omnidirectional band gap is in the B2 energy interval 2.4 - 4.2 eV. Colorbar corresponds to imaginary part of kz in m 1 units.. 4. ES Optimizer for Layered Structures Until now, our approach to designing structures with good reflection was based on band gap analysis. We stacked 18 segments of SiO 2 ZrO 2 with different periods in one structure to obtain reasonable performance. This is one possible way to design. However, it is not necesarily the best one and it is interesting to find out how close we are to the optimum. Different optimizers [17,18] can be helpful to find good solutions, that are often difficult to find analytically. If the structure consists of N layers, then there are N parameters (thickness of each layer) for the optimization. The search space should be defined for each parameter within a reasonable interval d min , d max . For such optimizations different evolutionary algorithms, like JEMAA.
(5) Design of Reflective, Photonic Shields for Atmospheric Reentry. 232. genetic algorithm (GA), micro-genetic algorithms (MGA), or evolutionary strategy (ES) may be applied. The optimization task becomes difficult, if there are many parameters for optimization, and/or if the fitness function has a complicated behavior with many local optima. We used ES for the optimization of our RPS. In previous applications ES usually outperformed GA and MGA. As an example of the ES approach, we maximized the average reflection R of the SiO 2 ZrO 2 structure containing N = 8 layers, at wavelength = 0.8 μm . Permittivities of SiO 2 and ZrO 2 are taken to be 1 = 2.1 and 2 = 4.8 at = 0.8 μm respectively. Layers are embedded between air interfaces. The average reflection to be optimized is defined as: R = R d1 , d 2 , , d8 = 0. π 2. Rs R p π. d ,. ( (a). (3). where Rs and R p are reflectivities for s- and p-polarized light respectively, di is the individual layer thickness, and is the angle of light incidence. The results of ES optimization are shown in Figure 6(a). Dashdotted curve corresponds to a Bragg mirror with layer thicknesses: d1 =. , d2 = . 4 1 4 2. (4). Dashed curve in the plot corresponds to an optimized Bragg mirror, with two optimized layer thicknesses. Solid line corresponds to a structure where all eight thicknesses are optimized. As seen from the plot, the optimization of all layer thicknesses (solid line) leads to the best performance. This reflects the fact that a Bragg mirror is not an optimal structure for omnidirectional reflection. A comparison of the layer thicknesses for three structures is shown in Figure 6(b).. 5. Optimization of the RPS Adjusted to One Energy Interval First we performed optimization of the RPS with respect to only one energy interval. Let us first consider RPS for the B1 energy interval. The fitness function to be optimized is defined in the expression (2). Band gap analysis revealed that 10 stacked periodic segments may cover this range with band gaps. The dashed line in Figure 8(a) shows reflectivity R1 as a function of the number of layers in this structure. In order to improve the reflec- tivity, we performed an ES structure optimization in two ways. In the first way, optimization was done in the full search space. This means that the thickness of each layer could have any value below d max = max 2n , max = 1.2 μm . This yields d max = 280 nm ( ZrO 2 ) and d max = 425 nm ( SiO 2 ). As mentioned earlier, optimiCopyright © 2011 SciRes.. (b). Figure 6. (a) Dash-dotted curve—reflectivity of the Bragg mirror, dashed curve—reflectivity of the optimized Bragg mirror, solid curve—reflectivity of the optimal structure. Wavelength λ = 0.8 μm (b) Thicknesses of individual layers for three structures, number of layers N = 8.. zation becomes demanding, if there are too many parameters for optimization and/or if the fitness function has a complicated behavior with many local optima. Therefore, it is helpful to visualize the dependence of the fitness function on the optimized parameters. Figure 7 shows the dependence of R1 (fitness) on the thicknesses of two arbitrary layers in the structure (4-th and 10-th layers are taken) containing 20 layers. One can see that the fitness function has a rather smooth behavior, which is advantageous for optimization. Moreover, smoothness of the fitness function means that the obtained solutions are quiet robust and small deviations (fabrication inaccuracies) in layer thicknesses will have a small impact on the reflectivity. Results of the optimization in the full search space are shown in Figure 8(a) (dash-dotted line). In our second optimization approach, we reduced the search space by using the thicknesses diseg of 10 stacked periodic segments as a first order approximation for the ES optimizer. Then we varied the thickness of. . . JEMAA.
(6) Design of Reflective, Photonic Shields for Atmospheric Reentry. 233. each layer in the range of d = 50,50 nm to obtain the optimum fitness. Thus, the obtained optimal thicknesses can be represented as: diopt = diseg di , i = 1, , N .. Figure 7.. R1. (fitness) of the structure as function of the. thicknesses of two layers (d4 and d10). Structure consists of 20 layers of SiO 2 ZrO 2 .. (5). Results for the optimization in the reduced search space are shown in Figure 8(a) (solid line). In both optimization procedures we restricted the number of fitness calls to 120,000 in order not to make the optimization very time-consuming. Of course, the reflectivity of the RPS can be further improved by means of simply increasing the time of optimization. Therefore, it should not be confusing that for N = 40 in Figure 8(a) dashdotted line is below the solid line. As seen in Figure 8(a), the structure optimization in the full search space (dash-dotted curve) becomes less efficient (time-consuming) for a high number of parameters N > 20 and the best performance comes from the optimized stacked segments. Thicknesses of individual layers for the three structures are compared in Figure 8(b). The improvement in reflectivity, however, is rather small and does not exceed 3% . We can therefore conclude that the stacked periodic segments is already a good solution for high reflection in B1 and only minor improvements can be achieved. A similar procedure was also performed for the second energy range B2 . Results are shown in Figure 9(b). 6. Optimization of the RPS Adjusted to Two Energy Intervals (a). (b). Figure 8. (a) Reflectivity. R1. as function of the number. of layers N in the structure. Dashed line—stacked periodic segments (periods from 200 to 425 nm), solid line—stacked segments optimized with ES, dash-dotted line—solution of the ES optimizer in the full search space. (b) Thicknesses of individual layers of the three structures, total number of layers is 20. Copyright © 2011 SciRes.. In a similar way we can optimize the reflection of RPS with respect to two energy intervals simultaneously. Now the fitness function to be optimized is R in the expression (1). Band gap analysis revealed that 18 stacked periodic segments may cover B1 and B2 intervals with band gaps. Again we can apply two approaches to perform the structure optimization using ES. The first approach is an optimization in the full search space, where the thickness of each layer is any value below d max = max 2n , max = 1.2 μm . However, as we saw in Section 5, this optimization procedure is not very efficient for many parameters N > 20 . So we used only the second ap- proach, which optimizes 18 stacked segments in the re- duced search space. We varied the thickness of each layer in the range [–30, 30] nm to find the optimum fitness. The obtained results are shown in Figure 10. As can be seen, optimization of 18 stacked segments (solid line) improves the reflecting performance. The improvement, however, is not large 3% for 36 layers and 0.5% for 72 layers. So, if the structure contains more than 36 layers, stacked periodic segments are close to the optimal solution for high reflectivity in the B1 and B2 energy intervals. JEMAA.
(7) Design of Reflective, Photonic Shields for Atmospheric Reentry. 234. (a). (a). (b). Figure 9. (a) Reflectivity. R2. of layers N in the structure. Dashed line—stacked periodic segments (periods from 90 to 180 nm), solid line—stacked segments optimized with ES, dash-dotted line—solution of the ES optimizer in the full search space. b) Thicknesses of individual layers of the three structures, total number of layers is 16.. For the sake of completeness, it is also worth plotting reflectivity spectra of the obtained structures. Up to now we plotted only the average values of reflectivity. Reflectivity as a function of energy of the stacked segments (dashed line) and optimized stacked segments (solid line) is shown in Figure 11. At each energy point reflectivity is averaged over angle of incidence . Dash-dotted line in Figure 11 is shown for the sake of comparison with the simple design, where two Bragg mirrors are stacked in one structure. Band gaps of these Bragg mirrors are centered in the middle of B1 and B2 intervals, the corresponding periods are 1 = 235 nm and 2 = 105 nm. A single Bragg mirror will partially cover only one interval ( B1 or B2 ). When Bragg mirrors are stacked together, both intervals are partially covered. Therefore, two peaks are observed in Figure 11. It is obvious that optimized segments (solid line) show the best reflecting performance. Copyright © 2011 SciRes.. (b). as function of the number Figure 10. (a) Reflectivity. R. of the structure for B1. and B2 energy intervals as function of the number of layers. Dashed line—stacked periodic segments, solid line—stacked segments optimized with ES. (b) Thicknesses of individual layers of the two structures, total number of layers N = 36.. Figure 11. Reflectivity R as function of energy. Dashed curve—18 stacked periodic segments, solid curve—18 stacked segments optimized with ES, dash-dotted curve— reflectivity of the stacked Bragg mirrors with periods 1 = 235 nm and 2 = 105 nm.. JEMAA.
(8) Design of Reflective, Photonic Shields for Atmospheric Reentry. 7. Possible Instabilities of the Designed Photonic Structure Due to High-Temperature Interaction of Individual Layers At high-temperatures, the interaction of ZrO 2 and SiO 2 layers (Figure 12) may be a source of dynamic instability in the position and width of the photonic band gap in designed photonic heat-shields. At temperature above 1300 C , irreversible reactions Equation (6) between of SiO 2 and ZrO 2 , will cause refractory zirconium orthosilicate ZrSiO 4 (zircon) interlayers to form at the interfaces SiO 2 ZrO 2 : SiO 2 ZrO 2 ZrSiO 4. (6). The upper limit of ZrSiO4 stability lies between 1669 and 1683˚C  which is close to the lowest eutectic temperature of 1687˚C. Reaction Equation (6) remains irreversible until 1550˚C at which point, a small fraction of ZrSiO 4 decays into constituent oxides. The rate of the ZrSiO 4 decomposition reaction increases at 1650˚C . The decay of ZrSiO 4 at 1673˚C was established based on an analysis of literature data, experimental results and thermodynamic assessments . The lowest eutectic in the system was established at the slightly higher temperature of 1687˚C . These results are in good agreement with DTA investigation of  where the zircon decomposition was determined to be at 1674˚C and the eutectic melting at 1680˚C. The preliminary literature analysis indicates that diffusivity of Si in SiO 2 [22,23] is several orders of magnitude higher than diffusivity of Si in ZrSiO 4  and Zr in ZrO 2 .. Figure 12. Scheme illustrating formation of ZrSiO4 interlayers as a result of high-temperature interaction SiO 2 ZrO 2 ZrSiO 4 under external heat radiation in the wavelength ranges B1 and B2. Thickness of intermediate ZrSiO 4 layers after exposure during operation time is much smaller than thickness of the SiO 2 and ZrO 2 layers d1 and d2 ( d1 , d 2 ) due to high activation energy of reaction of ZrSiO 4 formation. That is why erasing ZrSiO 4 interlayers do not change significantly position and width of the photonic band gaps of designed multilayers. Copyright © 2011 SciRes.. 235. Diffusivity of Zr in ZrSiO 4 is assumed to be similar to diffusivity of Hf in ZrSiO 4 , which is higher than diffusivity of Si . Among tetravalent cations, the diffusivity of Si in ZrSiO 4 is approximately the same as that of Ti but about one order of magnitude faster than diffusivity of Hf and two orders of magnitude faster than diffusivity of U and Th . A low speed of reaction Equation (6) and a small thickness of formed ZrSiO 4 interlayer after exposure time of the photonic heat-shield of approximately 300 sec are expected (see Figure 5 in , measurement of temperature response for standard PICA sample at 570 W/cm 2 , 0.42 atm, total heat load of 14’250 J cm 2 , surface temperature 2760 C ). Based on diffusion measurements, the activation energy of diffusion of Si in zircon was calculated , which is higher in comparison with other silicates. These data also confirm slow rates of reaction 6 at 1200˚C indicated by . The intermediate ZrSiO 4 layers consist of atoms of both contacted materials, and therefore, their dielectric permittivity has an intermediate value between the dielectric constants of ZrO 2 and SiO 2 materials. This affects reflection of light at the boundary. The influence of the intermediate layer on the transparency of photonic crystals has been considered in . It was found that the effect depends on the relation between the light wavelength and the interlayer thickness . Indeed, to estimate the effect, we can write the dielectric permittivity of the layer as a function of distance from the boundary = z (here z = 1 , if z < , but z = 2 , if z < ). The effect depends on the relation between the thickness of the layer ( ) and the light wavelength . Namely, the commonly used boundary conditions for the light wave fields hold at the abrupt boundary . This leads to the reflection and transmission coefficients used in this paper. On the contrary, at the smooth boundary we can use the semiclassical approximation and the wave equation with the position depen-dent wavelength z = 2πc ( z ) , which leads to the exponentially small reflectivity. Transition between these limiting cases for the similar quantum mechanical problem has been studied in [27,28]. Thus, the results presented here hold for , i.e. if the diffusion length is much smaller than the thickness of the layers we have deposed. Apparently, evolution of the interlayer thickness makes the reflectivity of the multilayer coating time-dependent. Nevertheless, the expected thickness of formed ZrSiO 4 interlayer should not exceed several lattice constants ( 2 10 nm) after heat-shield operation time. This is significantly smaller than the wavelength of external heat radiation in both B1 and B2 ranges and, therefore, does not change es- sentially the results of our modeling. It was found  that such small JEMAA.
(9) Design of Reflective, Photonic Shields for Atmospheric Reentry. 236. thickness of the ZrSiO 4 interlayer can change the depth, but not the position and width of the band gap of designed multilayer photonic structure.. 8. Conclusions Modeling layered SiO 2 ZrO 2 structure for potential use as photonic shield for Earth reentry was performed both analytically and numerically for shock layer radiation in near-IR and near-UV ranges. The analytical approach indicates that high omnidirectional reflectivity can be achieved by means of stacking 18 periodic segments in one structure. Optimization using evolutionary strategy resulted in structures with improved reflection performance. These structures demonstrate significantly enhanced reflectivity than a simple stack of two Bragg mirrors. The ES structure optimization method is quite general and can be used to design reflectors for other wavelength ranges without any restrictions on the constituent materials. High-temperature interactions at the SiO 2 ZrO 2 interface resulting in the formation of ZrSiO 4 interlayers is expected to be slow. Therefore, the interlayer is not expected to have a significant impact on the reflecting performance of the suggested multilayer coatings.. REFERENCES . . . V. Shklover, L. Braginsky, G. Witz, M. Mishrikey and C. Hafner, “High-Temperature Photonic Structures. Thermal Barrier Coatings, Infrared Sources and Other Applications,” Journal of Computational and Theoretical Nanoscience, Vol. 5, 2008, pp. 862-893. C. Johnston, B. Hollis and K. Sutton, “Spectrum Modeling for Air Shock-Layer Radiation at Lunar-Return Conditions,” Journal of Spacecraft and Rockets, Vol. 45, No. 5, 2008, pp. 865-878. doi:10.2514/1.33004 D. Bose, E. McCorkle, C. Thompson, D. Bogdanoff, D. Prabhu, G. Allen and J. Grinstead, “Analysis and Model Validation of Shock Layer Radiation in Air,” VKI LS Course on Hypersonic Entry and Cruise Vehicles, Palo Alto, 2008.. . C. Johnston, “A Comparison of EAST Shock-Tube Radiation Measurements with a New Air Radiation Model,” AIAA Paper 1245, 2008.. . J. Grinstead, M. Wilder, J. Olejniczak, D. Bogdanoff, G. Allen, K. Dang and M. Forrest, “Shock-Heated Air Radiation Measurements at Lunar Return Conditions,” AIAA Paper 1244, 2008.. . [Online]. Available: http://www.sopra-sa.com/.. . S. Venkataraj, R. Drese, C. Liesch, O. Kappertz, R. Jayavel and M. Wuttig, “Temperature Stability of Sputtered Niobium—Oxide Films,” Journal of Applied Physics, Vol. 91, No. 4863, 2002, pp. 61-68. doi:10.1063/1.1458052. . Y. Fink, J. Winn, S. Fan, C. Chen, J. Michel, J. Joan-. Copyright © 2011 SciRes.. nopoulos and E. Thomas, “A Dielectric Omnidirectional Reflector,” Science, Vol. 282, No. 5394, 1998, pp. 1679-1682. doi:10.1126/science.282.5394.1679 . E. Yablonovitch, “Engineered Omnidirectional External-Reflectivity Spectra from One-Dimensional Layered Interference Filters,” Optics Letters, Vol. 23, No. 21, 1998, pp. 1648-1649. doi:10.1364/OL.23.001648.  D. Chigrin, A. Lavrinenko, D. Yarotsky and S. Gaponenko, “Observation of Total Omnidirectional Reflection from a One-Dimensional Dielectric Lattice,” Applied Physics A: Materials Science & Processing, Vol. 68, No. 1, 1999, pp. 25-28. doi:10.1007/s003390050849  P. Yeh, “Optical Waves in Layered Media,” John Wiley & Sons, New York, 1988.  F. Kartner, N. Matuschek, T. Schibli, U. Keller, H. Haus, C. Heine, R. Morf, V. Scheuer, M. Tilsch and T. Tschudi, “Design and Fabrication of Double-Chirped Mirrors,” Optics Letters, Vol. 22, No. 11, 1997, pp. 831-833. doi:10.1364/OL.22.000831  T. Yonte, J. Monz´on, A. Felipe and L. S´anchez-Soto, “Optimizing Omnidirectional Reflection by Multilayer Mirrors,” Journal of Optics A: Pure and Applied Optics, Vol. 6, No. 1, 2004, pp. 127-131. doi:10.1088/1464-4258/6/1/023  M. del Rio and G. Pareschi, “Global Optimization and Reflectivity Data Fitting for X-Ray Multilayer Mirrors by Means of Genetic Algorithms,” Proceedings of SPIE, Vol. 4145, No. 88, 2001, p. 88. doi:10.1117/12.411624  S. Martin, J. Rivory and M. Schoenauer, “Synthesis of Optical Multilayer Systems Using Genetic Algorithms,” Applied Optics, Vol. 34, No. 13, 1995, pp. 2247-2254. doi:10.1364/AO.34.002247  J. Joannopoulos, S. Johnson, J. Winn and R. Meade, “Photonic Crystals: Molding the Flow of Light,” Princeton University, Princeton, 2008.  A. Fallahi, M. Mishrikey, C. Hafner and R. Vahldieck, “Efficient Procedures for the Optimization of Frequency Selective Surfaces,” IEEE Transactions on Antennas and Propagation, Vol. 56, No. 5, 2008, p. 1340. doi:10.1109/TAP.2008.922678  C. Hafner, C. Xudong, J. Smajic and R. Vahldieck, “Efficient Procedures for the Optimization of Defects in Photonic Crystal Structures,” Journal of the Optical Society of America A, Vol. 24, No. 4, 2007, pp. 1177-1188. doi:10.1364/JOSAA.24.001177  A. Kaiser, M. Lobert and R. Telle, “Thermal Stability of Zircon (ZrSiO4),” Journal of the European Ceramic Society, Vol. 28, No. 11, 2008, pp. 2199-2211. doi:10.1016/j.jeurceramsoc.2007.12.040  W. Butterman and W. Foster, “Zircon Stability and the ZrO2-SiO2 Phase Diagram,” American Mineralogist, Vol. 52, 1967, pp. 880-885.  D. Kamaev, S. Archugov and G. Mikhailov, “Study and Thermodynamic Analysis of the ZrO2-SiO2 System,” Russian Journal of Applied Chemistry, Vol. 78, No. 2, 2005, pp. 200-203. doi:10.1007/s11167-005-0259-2  F. B’ejina and O. Jaoul, “Silicon Diffusion in Silicate. JEMAA.
(10) Design of Reflective, Photonic Shields for Atmospheric Reentry Minerals,” Earth and Planetary Science Letters, Vol. 153, No. 3-4, 1997, pp. 229-238. doi:10.1016/S0012-821X(97)00190-8  D. Tsoukalas, C. Tsamis and P. Normand, “Diffusivity Measurements of Silicon in Silicon Dioxide Layers Using Isotopically Pure Material,” Journal of Applied Physics, Vol. 89, No. 12, 2001, pp. 7809-7813. doi:10.1063/1.1371003  D. Cherniak, “Si Diffusion in Zircon,” Physics and Chemistry of Minerals, Vol. 35, No. 4, 2008, pp. 179-187. doi:10.1007/s00269-007-0210-6  H. Drings, U. Brossmann, H. Carstanjen, A. Szokefalvi-Nagy, C. Noll and H. Schaefer, “Enhanced 95Zr Diffusion in Grain Boundaries of Nano-Crystalline ZrO2. Copyright © 2011 SciRes.. 237. 9.5 mol% Y2O3,” Physica Status Solidi (A), Vol. 206, No. 1, 2008, pp. 54-58. doi:10.1002/pssa.200824077  L. Braginsky and V. Shklover, “Light Propagation in an Imperfect Photonic Crystal,” Physical Review B, Vol. 73, No. 8, 2006. doi:10.1103/PhysRevB.73.085107  E. Baskin and L. Braginsky, “Short-Wavelength Phonon Emission from a Metal-Semiconductor Interface,” Physical Review B, Vol. 50, No. 16, 1994, pp. 12191-12194. doi:10.1103/PhysRevB.50.12191  L. Braginsky and V. Shklover, “Influence of Interface Structure on Transversal Electron Transport,” Solid State Communications, Vol. 105, No. 11, 1998, pp. 701-704. doi:10.1016/S0038-1098(97)10209-5. JEMAA.